Analyse SAXS de traces ioniques causées par bombardements d’ions d’or dans des échantillons de silicium amorphe
The following thesis aims to verify whether the formation of latent traces by heavy and fast ions passes through a liquid phase. Given the fact that the process of trace formation is too fast to be directly studied, our experience aims to measure after the fact elements that would be indicative of a merger. In this context, we will study whether there has been a redistribution of gold ions (initially present by doping in amorphous silicon samples) following the irradiation of the samples. This redistribution of gold could be explained by the phenomenon of refining the melted zone, which would occur during a rise in temperature during the creation of latent ionic traces predicted by the theoretical model of the thermal peak.  The samples studied are amorphous silicon membranes of 2 µm in thickness, doped with gold at different percentages (pure, medium and high) and irradiated with fast heavy ions of gold at 1.1 GeV or silver at 75 MeV.  No SAXS image was able to reveal the presence of latent ionic traces for samples irradiated with silver ions at 75 MeV. Although the stopping power of the latter is low (9.5 keV/nm), it exceeds the threshold observed for several other phenomena associated with traces. [2] [3] We would therefore have found a regime where there are effects of heavy and fast ions, but without a visible signature in SAXS.  In contrast, irradiated samples of gold ions demonstrated the presence of latent ionic traces via SAXS images. These images demonstrate a diffusion pattern characteristic of core-shell type traces. However, these results do not show differences in gold segregation according to the initial doping level. All samples (pure, medium and high doping) have a core radius of (2.5 ± 0.1) nm and a total radius of (9.9 ± 0.5) nm, which are values similar to those obtained in the literature. [4] On the other hand, the absence of a difference according to the doping could be explained by the fact that the resolidification after the fusion would be too fast, to the point where the gold would undergo solute trapping which would prevent the segregation. Another possible explanation would be that there would be no fusion at all during the formation of the trace.  First of all, this thesis deals with all the steps necessary for the design of the samples, namely their amorphization, the implantation of gold impurities, then the irradiation. Two categories of samples are discussed: the validation samples, then the actual samples that were studied. Subsequently, this thesis addresses the detection of latent ion traces, first with an AFM (which proved to be insufficient), then with SAXS measurements. Finally, a theoretical code to reproduce the experimental measurements obtained was developed based on the literature. It generates promising numerical results compared to the experimental data obtained.
HF or SAXS form factor gold latent ion track zone reﬁning Amorphous silicon